- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

International Journal of Photoenergy

Volume 2012 (2012), Article ID 858350, 7 pages

http://dx.doi.org/10.1155/2012/858350

## Current Mechanism in -Gated Metal-Oxide-Semiconductor Devices

Department of Physics, Faculty of Sciences and Arts, Batman University, 72000 Batman, Turkey

Received 9 January 2012; Revised 27 March 2012; Accepted 10 April 2012

Academic Editor: Xie Quan

Copyright © 2012 Osman Pakma. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The present study aimed to examine the current density-voltage (*J-V*) characteristics of Al/HfO_{2}/p-Si (MOS) structure at temperatures ranging between 100 and 320 K and to determine the structure’s current transport mechanism. The HfO_{2} film was coated on a single side of the p-Si (111) crystal using the spin coating method. The *J-V* measurements of the obtained structure at the temperatures between 100 and 320 K revealed that the current transport mechanism in the structure was compatible with the Schottky emission theory. The Schottky emission theory was also used to calculate the structure’s Schottky barrier heights (), dielectric constants () and refractive index values of the thin films at each temperature value. The dielectric constant and refractive index values were observed to decrease at decreasing temperatures. The capacitance-voltage (*C-V*) and conductance-voltage (*G/ ω-V*) characteristics of Al/HfO

_{2}/p-Si (MOS) structure was measured in the temperature range of 100–320 K. The values of measured

*C*and

*G/*decrease in accumulation and depletion regions with decreasing temperature due to localized at Si/HfO

*ω*_{2}interface.

#### 1. Introduction

As an important group of thin-film electronic materials for microelectronics, dielectrics have a broad range of device applications. They are instrumental both in active devices like transistors and their electrical isolation and in passive devices like capacitors. In these days, when Si-based device technologies are widely put to use, thin film dielectric materials have properties that could be useful in many areas. They have recently been used in both high-permittivity applications such as transistor gate and capacitor dielectrics and low-permittivity materials like inter-level metal dielectrics which operate at switching frequencies in the gigahertz regime for the most demanding applications.

For over forty years, silicon dioxide (SiO_{2}) films have been preferred for gate dielectric in metal-oxide-semiconductor (MOS) devices. SiO_{2} films get thinner in smaller MOS devices. Currently, the technology is aiming to obtain node technologies thinner than 100 nm [1], to which an SiO_{2} gate oxide thickness of 1.5–2 nm corresponds. Since direct tunneling has to be made through the thin oxide, high leakage current and reliability problems occur. The solution is high dielectric materials. A good example for future MOS technologies is HfO_{2}, while a thickness less than 100 nm in silicon demands a gate dielectric other than SiO_{2} [2]. With a high dielectric constant (20–25) and a high band gap (5.1–6.0 eV) [3, 4], it is compatible with polycrystalline silicon gate process and is also thermally stable with silicon [5]. The methods used to prepare HfO_{2} thin films have a wide variety. To mention a few, they include Rf magnetron sputtering [6], chemical vapor deposition, and sol-gel process [7, 8]. Of all these methods, the sol-gel method is among the most promising ones because this method could easily control the optical and other properties of thin film when the solution composition and deposition condition are changed.

Thin Hf-layer-coated structures have been reported to include various types of current transport mechanisms, which are Fowler-Nordheim (FN) tunneling, trap-assisted tunneling (TAT), Schottky emission, Poole-Frenkel (PF), direct tunneling (DT), and tunneling-assisted PF emission (TAPF). Pan et al. performed current-voltage (*I-V*) measurements at high temperatures on HfO_{2}/TaN-based metal-insulator-metal (MIM) structures whose HfO_{2} dielectric material was prepared using the atomic-layer-deposition (ALD) method, and on the basis of their measurements, they demonstrated that the Schottky emission current dominates in the low-field range of this structure, while the Poole-Frenkel (PF) emission current dominates in its high-field range [9]. As a result of their *I-V* measurements on Al/HfO_{2}/p-Si metal-oxide-semiconductor structures whose HfO_{2} dielectric material was prepared by the RF magnetron sputtering method, Chiu and colleagues reported that the Schottky emission current dominates in the structure at high temperatures and in low-field range, whereas Fowler-Nordheim (FN) tunneling dominates at low temperatures and in high-field range [10].

The present study examined the *I-V* characteristics in a temperature range of 100–320 K of Al/HfO_{2}/p-Si (MOS) structure whose HfO_{2} thin film was prepared by the sol-gel immersion method.

#### 2. Design and Fabrication of Al/HfO_{2}/p-Si Structures

To prepare the HfO_{2} solution, 0.0063 mol hafnium tetrachloride was dissolved in 15 mL ethanol, to which 0.08 mol H_{2}O and 0.013 mol HNO_{3} were added and the solution was kept in a magnetic stirrer for 2 hours. Finally, before coating the film, the solution was kept at 50°C for 4 hours. Several metal-oxide-semiconductor (Al/HfO_{2}/p-Si) structures were fabricated on the 3-inch diameter float zone <111> p-type (boron-doped) single crystal silicon wafer with a thickness of 600 *μ*m and a resistivity of 5–10 Ωcm. For the fabrication process, Si wafer was degreased through the RCA cleaning procedure (i.e., a 10-minute boiling in NH_{4}OH + H_{2}O_{2} + 6 DI (18 MΩ deionised water), which was followed by a 10-minute boiling in HCl + H_{2}O_{2} + 6 DI) [11]. Next, it was subjected to the drying process in N_{2} atmosphere for a prolonged time. Following the drying process, high-purity aluminum with a thickness of 1500 was thermally evaporated from the tungsten filament onto the whole back surface of the Si wafer under the pressure of 10^{−7} Torr. In order to obtain a low-resistivity ohmic back contact, Si wafer was sintered at 580°C for 3 minutes in N_{2} atmosphere. The native oxide on the front surface of the substrate was removed in HF : H_{2}O (1 : 10) solution, and finally, the wafer was rinsed in deionised water for 30 s before forming an organic layer on the p-type Si substrate. The prepared HFO_{2} solution was coated on the shiny side of the cleaned p-Si surface at 2000 rpm by the sol-gel spinning technique. The HfO_{2}/p-Si structure was annealed for five minutes at 300°C in N_{2} atmosphere after each coating process. The procedure was repeated in the same way until the required film thickness was obtained and the structure was finally subjected to annealing at 500°C in N_{2} atmosphere for 1 h. The interfacial oxide layer thickness was estimated to be about 8.9 nm by spectroscopic ellipsometry (VASE M2000). In order to obtain a rectifying contact on the front surface of p-Si coated with HfO_{2, }a high-purity aluminum layer was coated on the surface in a high vacuum under the pressure of 10^{−7} Torr. The Al/HfO_{2}/p-Si (MOS) structure is given in Figure 1. The current-voltage (*I-V*) characteristics of the samples were measured in the temperature range of 100–320 K using a temperature controlled Janis CCS-350S cryostat, which allowed us to perform the measurements in the temperature range of 10–325 K, and using a Keithley 2420 programmable constant current source under dark conditions. The sample temperature was continually monitored using a GaAlAs sensor and a Lakeshore 330 auto-tuning temperature controller with a sensitivity better than ±0.1 K. The forward and reverse bias capacitance-voltage (*C-V*) and conductance-voltage (*G-V*) measurements were performed in the 1 MHz by using an HP 4192 A LF impedance analyzer (5 Hz to 13 MHz) and the test signal of 50 mV_{rms}. All measurements were carried out in the temperature range of 100–320 K and in the dark.

#### 3. Measurement and Experimental Results

Figure 2 presents the current density-voltage (*J-V*) characteristics of the Al/HfO_{2}/p-Si (MOS) structure measured in the temperature range of 100–320 K and from −3 V to +3 V. It is found that reverse leakage current density at −1 V is 5.63 × 10^{−4} A/cm^{2} for 100 K and 1.35 × 10^{−2} A/cm^{2} for 320 K, respectively. The reverse bias leakage current was observed to be 26 times higher at 320 K than that of 100 K. It is noted that the leakage current increases with increase in temperature. As can be seen in this figure, the ln*J-V* plots are linear on a semilogarithmic scale at low forward bias voltages but deviate considerably from linearity at high forward bias voltages due to the effect of series resistance on the interfacial insulator layer (HfO_{2}). The current density across an ideal Schottky barrier diode (SBD), based on the thermionic emission (TE) theory, is given by the following relation () [12]:
where is the reverse saturation current density:
where , , *, **, **, *and are the zero bias barrier height, series resistance of structure, the effective Richardson constant (32 A/cm^{2} K^{2} for p-type Si [12]), the ideality factor, the electron charge, and the temperature in Kelvin, respectively.

As it is known, the characteristic ln*J-V* graph of a diode usually has three regions, which are low-voltage region ( V), medium-voltage region (0.1 V 0.8 V), and high-voltage region ( V), respectively. The electrical parameters except for were calculated in the linear region in the medium voltage region, while was calculated in the region where the ln*J-V* curve in the high-voltage region bended. As can be seen from Figure 2, each semilogarithmic *J-V* curve consists of a linear range with different slopes in between the intermediate-bias voltage () regions. The experimental values of and were determined from (1) and (2), respectively, and they are shown at each temperature in Table 1. As can be seen in Table 1, the values of and range from 1.24 and 0.516 eV (320 K) to 4.32 and 0.172 eV (100 K), respectively. Both parameters exhibit a strong temperature dependency as seen in Figure 3. As seen from Figure 3, while increased, decreased with decreasing temperature. Because of the temperature-activated process, the current transport will be dominated by current flowing through the lower BH and a larger ideality factor [13]. That is, more electrons have sufficient energy to overcome the higher barrier when temperature increases, and then, BH increases with temperature and bias voltage.

Figure 4 shows the conventional Richardson (ln() versus 1/*T* plot. The Richardson constant and effective barrier height at 0 K are obtained from the intercept and slope of linear fit. ln() versus 1/*T *plot has two linear temperature ranges. In the first region (180–320 K), the values of effective barrier height obtained from the slope of this straight line come out to be 0.096 eV. Likewise, the value Richardson constant determined from the intercept at the ordinate is 2.52 × 10^{−7} A/cm^{2} K^{2}. In the second region (100–160 K), the values of effective barrier height and Richardson constant were derived from the slope and intercept of this straight line as 0.0013 eV and 6.01 × 10^{−10} A/cm^{2} K^{2}, respectively. The Richardson constant values are much lower than the known value of 32 A/cm^{2} K^{2} for p-type Si. As explained before, the deviation in the Richardson plots might be a result of the spatially inhomogeneous barrier heights and potential fluctuations at the interface, which consist of low and high barrier areas [14–17].

Figure 5 shows a plot of the experimental barrier height versus the ideality factor for various temperatures. As can be seen in Figure 5, there are linear regions between the experimental barrier heights and ideality factors of the Al/HfO_{2}/p-Si (MOS) structure, which can be explained by lateral inhomogeneities of the barrier heights [14, 17]. The exploration of the experimental barrier height versus the ideality factor plot to has given a value of 0.503 eV, which is close to half of the band gap in Si. These results confirm that the predominant current transport is not the TE in our samples.

The standard Schottky emission equation is as follows [12]:
where (A/cm^{2}K^{2}), is the effective Richardson constant, is the electronic charge, is the electric field, is Planck’s constant, is the permittivity of free space, is the dynamic dielectric constant, is the free electron mass, and is the electron effective mass in HfO_{2} ( = 0.4 for Al/HfO_{2} and = 0.18 for HfO_{2}/Si) [5, 18].

For the standard Schottky emission, a plot of ln() versus should be linear. As seen in Figures 6 and 7, there is a very good fit between the experimental data in the region for each measurement temperature and high electric field and the Schottky emission theory for both gate injection and substrate injection. At each temperature in Table 2, the experimental refractive index values , and were determined from (3), respectively. Table 2 reveals that experimentally determined dynamic dielectric constants at room temperature in standard Schottky plots are so close to 4, the square of the refractive index 2 [3, 19]. This points out to the consistency between the conduction mechanism under high electric fields and Schottky emission. Another observation was that the extracted refractive index value gradually increases with increased measurement temperature, which may result from the effects of thermal stress, thermal expansion, and electronic polarizability [20–22]. The barrier height at the Al/HfO_{2} and HfO_{2}/p-Si interfaces was determined from 0.482 and 0.342 eV (100 K) to 0.936 and 0.778 eV (320 K), respectively.

There are a number of suggested methods which help to extract the of structure, and among them the most important one is the conductance method, developed by Nicollian and Goetzberger [23–26]. In this method, the frequency-dependent forward and reverse bias *C-V *and *G/ ω-V* measurements give the detail information on the distribution profile of of MOS structure. When the MOS structure is biased into strong accumulation, the impedance is given by [23]
where and are the measured capacitance and conductance, in strong accumulation region. Series resistance is the real part of the impedance () or
The oxide layer capacitance () is obtained by substituting from (5) into the following relations:
where and are the capacitance and conductance measured across the MOS structure at any bias voltage.

The capacitance-voltage (*C-V*) and conductance-voltage (*G/ ω-V*) characteristics of Al/HfO

_{2}/p-Si (MOS) structure were measured in the temperature range of 100–320 K (1 MHz) and are given in Figures 8(a) and 8(b), respectively. As can be seen from Figures 8(a) and 8(b) both curves have three distinct regimes of accumulation-depletion-inversion. The values of measured and

*G/*decrease in accumulation and depletion regions with decreasing temperature due to localized at Si/HfO

*ω*_{2}interface. Such behavior of the and

*G/*is attributed to particular distribution of interface states at p-Si/HfO

*ω*_{2}interfaces and of structure [23].

Using (5) the values of were calculated as a function of bias in the temperature range of 100–320 K and are given in Figure 9. As can be clearly seen from Figure 9, the gives a peak. The peak position of is shifting toward inversion region with increasing temperature. Such behavior of is attributed to the particular distribution of localized at p-Si/HfO_{2} interface states and interfacial insulator layer at Al/p-Si interface.

The density of interface states () at p-Si/HfO_{2} can be derived from Hill-Coleman method [27]. According to this method, is given by
where is the area of the structure, and is the maximum measured conductance value. Figure 10 shows that the increase with increasing temperature. The high values of and at high temperatures were attributed to the excess capacitance resulting from the , which is in equilibrium with the semiconductor that follows the ac signal.

#### 4. Conclusions

The forward and reverse *J-V*, *C-V,* and *G/ ω-V* characteristics of Al/HfO

_{2}/p-Si (MOS) structure derived using the sol-gel method were measured at temperatures ranging between 100 and 320 K. The

*J-V*measurements of the obtained Al/HfO

_{2}/p-Si (MOS) structure at the temperatures between 100 and 320 K revealed that the current transport mechanism in the structure was compatible with the Schottky emission theory. The Schottky emission theory was also used to calculate the structure’s Schottky barrier heights (), dielectric constants (), and refractive index values of the thin films at each temperature value. The dielectric constant and refractive index values were observed to decrease at decreasing temperatures. The values of measured and

*G/*decrease in accumulation and depletion regions with decreasing temperature due to localized at Si/HfO

*ω*_{2}interface. The increase with increasing temperature.

#### References

- R. K. Nahar, V. Singh, and A. Sharma, “Study of electrical and microstructure properties of high dielectric hafnium oxide thin film for MOS devices,”
*Journal of Materials Science*, vol. 18, no. 6, pp. 615–619, 2007. View at Publisher · View at Google Scholar · View at Scopus *International Technology Road Map for Semiconductors*, San-Jose, Calif, USA, 1999.- M. Balog, M. Schieber, M. Michman, and S. Patai, “Chemical vapor deposition and characterization of HfO
_{2}films from organo-hafnium compounds,”*Thin Solid Films*, vol. 41, no. 3, pp. 247–259, 1977. View at Scopus - M. Housa,
*High k Gate Dielectric*, IPO, Bristal, 2004. - F. C. Chiu, “Interface characterization and carrier transportation in metal/ HfO
_{2}/silicon structure,”*Journal of Applied Physics*, vol. 100, no. 11, Article ID 114102, 2006. View at Publisher · View at Google Scholar · View at Scopus - L. Khomenkova, X. Portier, J. Cardin, and F. Gourbilleau, “Thermal stability of high-k Si-rich HfO
_{2}layers grown by RF magnetron sputtering,”*Nanotechnology*, vol. 21, no. 28, Article ID 285707, 2010. View at Publisher · View at Google Scholar · View at Scopus - Y. Ohshita, A. Ogura, A. Hoshino, S. Hiiro, T. Suzuki, and H. Machida, “Using tetrakis-diethylamido-hafnium for HfO
_{2}thin-film growth in low-pressure chemical vapor deposition,”*Thin Solid Films*, vol. 406, no. 1-2, pp. 215–218, 2002. View at Publisher · View at Google Scholar · View at Scopus - Y. Aoki, T. Kunitake, and A. Nakao, “Sol-gel fabrication of dielectric HfO
_{2}nano-films; formation of uniform, void-free layers and their superior electrical properties,”*Chemistry of Materials*, vol. 17, no. 2, pp. 450–458, 2005. View at Publisher · View at Google Scholar · View at Scopus - S. Pan, S. J. Ding, Y. Huang et al., “High-temperature conduction behaviors of HfO
_{2}/TaN-based metal-insulator-metal capacitors,”*Journal of Applied Physics*, vol. 102, no. 7, Article ID 073706, 2007. View at Publisher · View at Google Scholar · View at Scopus - F. C. Chiu, S. A. Lin, and J. Y. M. Lee, “Electrical properties of metal-HfO
_{2}-silicon system measured from metal-insulator-semiconductor capacitors and metal-insulator-semiconductor field-effect transistors using HfO_{2}gate dielectric,”*Microelectronics Reliability*, vol. 45, no. 5-6, pp. 961–964, 2005. View at Publisher · View at Google Scholar · View at Scopus - W. Kern,
*Handbook of Semiconductor Cleaning Technology*, Noyes, New York, NY, USA, 1993. - S. M. Sze and K. Ng Kwok,
*Physics of Semiconductor Devices*, Wiley, Hoboken, NJ, USA, 3nd edition, 2007. - R. F. Schmitsdorf, T. U. Kampen, and W. Mönch, “Explanation of the linear correlation between barrier heights and ideality factors of real metal-semiconductor contacts by laterally nonuniform Schottky barriers,”
*Journal of Vacuum Science and Technology B*, vol. 15, no. 4, pp. 1221–1226, 1997. View at Scopus - Ş. Karataş, Ş. Altindal, A. Türüt, and A. Özmen, “Temperature dependence of characteristic parameters of the H-terminated Sn/p-Si(1 0 0) Schottky contacts,”
*Applied Surface Science*, vol. 217, no. 1–4, pp. 250–260, 2003. View at Publisher · View at Google Scholar · View at Scopus - E. Dobročka and J. Osvald, “Influence of barrier height distribution on the parameters of Schottky diodes,”
*Applied Physics Letters*, vol. 65, no. 5, pp. 575–577, 1994. View at Publisher · View at Google Scholar · View at Scopus - F. E. Jones, B. P. Wood, J. A. Myers, C. Daniels-Hafer, and M. C. Lonergan, “Current transport and the role of barrier inhomogeneities at the high barrier
*n*-InP ∣ poly(pyrrole) interface,”*Journal of Applied Physics*, vol. 86, no. 11, pp. 6431–6441, 1999. View at Scopus - M. C. Lonergan and F. E. Jones, “Calculation of transmission coefficients at nonideal semiconductor interfaces characterized by a spatial distribution of barrier heights,”
*Journal of Chemical Physics*, vol. 115, no. 1, pp. 433–445, 2001. View at Publisher · View at Google Scholar · View at Scopus - Y. T. Hou, M. F. Li, H. Y. Yu, and D. L. Kwong, “Modeling of tunneling currents through HfO
_{2}and (HfO_{2})_{x}(Al_{2}O_{3})_{1-x}gate stacks,”*IEEE Electron Device Letters*, vol. 24, no. 2, pp. 96–98, 2003. View at Publisher · View at Google Scholar · View at Scopus - H. W. Chen, F. C. Chiu, C. H. Liu et al., “Interface characterization and current conduction in HfO
_{2}-gated MOS capacitors,”*Applied Surface Science*, vol. 254, no. 19, pp. 6112–6115, 2008. View at Publisher · View at Google Scholar · View at Scopus - W. H. Cheng, S. F. Chi, and A. K. Chu, “Effect of thermal stresses on temperature dependence of refractive index for Ta
_{2}O_{5}dielectric films,”*Thin Solid Films*, vol. 347, no. 1-2, pp. 233–237, 1999. View at Publisher · View at Google Scholar · View at Scopus - C. Z. Tan, “Review and analysis of refractive index temperature dependence in amorphous SiO
_{2},”*Journal of Non-Crystalline Solids*, vol. 238, no. 1-2, pp. 30–36, 1998. View at Scopus - S. J. Ding, J. Xu, Y. Huang, Q. Q. Sun, D. W. Zhang, and M. F. Li, “Electrical characteristics and conduction mechanisms of metal-insulator-metal capacitors with nanolaminated Al
_{2}O_{3}-HfO_{2}dielectrics,”*Applied Physics Letters*, vol. 93, no. 9, Article ID 092909, 2008. View at Publisher · View at Google Scholar · View at Scopus - E. H. Nicollian and J. R. Brews,
*Metal-Oxide Semiconductor (MOS) Physics and Technology*, Wiley, New York, NY, USA, 1982. - H. Norde, “A modified forward I-V plot for Schottky diodes with high series resistance,”
*Journal of Applied Physics*, vol. 50, no. 7, pp. 5052–5053, 1979. View at Publisher · View at Google Scholar · View at Scopus - K. Sato and Y. Yasumura, “Study of forward I-V plot for Schottky diodes with high series resistance,”
*Journal of Applied Physics*, vol. 58, no. 9, pp. 3655–3657, 1985. View at Publisher · View at Google Scholar · View at Scopus - S. K. Cheung and N. W. Cheung, “Extraction of Schottky diode parameters from forward current-voltage characteristics,”
*Applied Physics Letters*, vol. 49, no. 2, pp. 85–87, 1986. View at Publisher · View at Google Scholar · View at Scopus - W. A. Hill and C. C. Coleman, “A single-frequency approximation for interface-state density determination,”
*Solid-State Electronics*, vol. 23, no. 9, pp. 987–993, 1980. View at Scopus